- About this Journal ·
- Abstracting and Indexing ·
- Advance Access ·
- Aims and Scope ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

Advances in Condensed Matter Physics

VolumeÂ 2010Â (2010), Article IDÂ 167985, 6 pages

http://dx.doi.org/10.1155/2010/167985

## The Phenomenology of Iron Pnictides Superconductors Explained in the Framework of -Wave Three-Band Eliashberg Theory

Dipartimento di Fisica and CNISM, Politecnico di Torino, Corso Duca degli Abruzzi 24, 10129 Torino, Italy

Received 25 May 2009; Revised 10 August 2009; Accepted 3 September 2009

Academic Editor: IgorÂ Mazin

Copyright Â© 2010 G. A. Ummarino. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

The *s*-wave three-band Eliashberg theory can simultaneously reproduce the experimental critical temperatures and the gap values of the superconducting materials , and as exponent of the more important families of iron pnictides. In this model the dominant role is played by interband interactions and the order parameter undergoes a sign reversal between hole and electron bands (-wave symmetry). The values of all the gaps (with the exact experimental critical temperature) can be obtained by using high values of the electron-boson coupling constants and small typical boson energies (in agreement with experiments).

The discovery of Fe-based pnictide superconductors [1â€“3] has aroused great interest in the scientific community. For the first time noncuprate superconductor shows high critical temperature. In these systems, as in cuprates, the superconductivity occurs upon charge doping of a magnetic parent compound above a certain critical value. The more relevant difference is that in cuprates the parent compound is a Mott insulator with localized charge carriers and a strong Coulomb repulsion between electrons, while in the pnictides it is a bad metal and shows a tetragonal to orthorhombic structural transition below 140 K, followed by the onset of an antiferromagnetic spin-density-wave ordering [4]. Charge doping gives rise to superconductivity and, at the same time, inhibits the occurrence of both the static magnetic order and the structural transition. The Fermi surface consists of two or three hole-like sheets around the point in the first Brillouin zone and two electron-like sheets around point. Up to now, the most intensively studied systems are the 1111 compounds, ReFeAs (Re = La, Sm, Nd, Pr, etc.) and the 122 ones, hole- or electron-doped AFA (A = Ba, Sr, Ca).

At present it is not completely clear what is the microscopic pairing mechanism responsible for superconductivity. The conventional phonon-mediated coupling mechanism is too week and cannot explain the observed high within the standard Migdal-Eliashberg theory [5, 6]. The calculated increases only marginally with the inclusion of multiband effects and remains far from experimental values. On the other hand, the magnetic nature of the parent compound seems to favor a coupling mechanism based on nesting-related antiferromagnetic spin fluctuations [7]. In this case an interband sign reversal of the order parameter between different sheets of the Fermi surface ( symmetry) is predicted. The number, amplitude, and symmetry of the superconducting energy gaps are indeed fundamental physical quantities that any microscopic model of superconductivity has to account for. Experiments with powerful techniques such as ARPES, point-contact spectroscopy, and STM, have been carried out to study the superconducting gaps in pnictides (for a review see [8]). Although the results are sometimes in disagreement with each other, a multigap scenario is emerging with evidence for rather high gap ratios, [8]. A two-band BCS model cannot account either for the amplitude of the experimental gaps or for their ratio. Three-band BCS models have been investigated [9â€“11] which can reproduce the experimental gap ratio but not the exact experimental gap values when the experimental is exactly reproduced. In this regard, a reliable study has to be carried out within the framework of the Eliashberg theory for strong coupling superconductors [12â€“18], due to the possible high values of the coupling constants necessary to explain the experimental data.

By using this strong-coupling approach, I show here that the superconducting iron pnictides represent a case of dominant negative interband-channel superconductivity (-wave symmetry) with high values of the electron-boson coupling constants and small typical boson energies. Furthermore I prove that a small contribution of intraband coupling does not significantly affect the obtained results and that the contribution of the Coulomb pseudopotential is negligible.

The electronic structure of pnictides can be approximately reproduced by using a three-band model (Figure 1) with two hole bands (1 and 2) and one equivalent electron band (3) [9]. The -wave order parameters of the hole bands and have opposite sign with respect to that of the electron [7]. In such systems intraband coupling could be provided by phonons while interband coupling by antiferromagnetic spin fluctuations which in a one-band system are always pair breaking but here, in a multiband system, the interband terms can contribute to increase the critical temperature. In the multiband Eliashberg equations the spin fluctuations term in the intraband channel has positive sign for the renormalization functions and negative sign for the superconducting order parameters thus leading to a strong reduction of . However, if we consider negative interband contributions in the equations, the final result can be an increase of the critical temperature [19].

The generalization of the Eliashberg theory [12â€“18] for multiband systems has already been used with success to study the MgB superconductor [20â€“23]. To obtain the gaps and the critical temperature within the -wave, three-band Eliashberg equations, one has to solve six coupled equations for the gaps and the renormalization functions , where is a band index that ranges between and (see Figure 1) and are the Matsubara frequencies. For completeness we included in the equations the nonmagnetic and magnetic impurity scattering rates in the Born approximation, and . In the imaginary-axis formulation [24] the equations are

where , . is the Heaviside function and is a cut-off energy. In particular, , where means â€śphononâ€ť and â€śspin fluctuations.â€ť Finally, and .

In the real axis formulation the multiband -wave Eliashberg equations [25, 26] are

where now , . In particular, , and and .

In principle the solution of the three-band Eliashberg equations shown in (1) (or (2)) requires a huge number of input parameters: (i) nine electron-phonon spectral functions, ; (ii) nine electron-SF spectral functions, ; (iii) nine elements of the Coulomb pseudopotential matrix, ; (iv) nine nonmagnetic and nine paramagnetic impurity scattering rates.

It is obvious that a practical solution of these equations requires a drastic reduction in the number of free parameters of the model. According to the work of Mazin et al. [7] I know that (i) that is, phonons mainly provide intraband coupling but the total electron-phonon coupling constant should be very small [5, 6], (ii) , that is, SF mainly provide interband coupling. I include these features in the simplest three-band model by posing , , and . Here, of course, it is . Moreover, I set in (1)-(2) and (3)-(4).

Within these approximations, the electron-boson coupling-constant matrix becomes [9]

where , , and is the normal density of states at the Fermi level for the -band ( according to Figure 1).

I initially solved the Eliashberg equations on the imaginary axis to calculate the critical temperature and, by means of the technique of the PadĂ¨ approximants [27, 28], to obtain the low-temperature value of the gaps because in presence of a strong coupling interaction or of impurities, the value of obtained by solving the imaginary-axis Eliashberg equations can be very different from the value of obtained from the real-axis Eliashberg equations [29]. I also solved the three-band Eliashberg equations in the real-axis formulation.

I reproduced the critical temperature and the gap values in three representative cases: (i) the compound LaFeAsOF with â€‰K where point-contact spectroscopy measurements gave meV and â€‰meV [30]; (ii) the compound BaKFeAs with K where ARPES measurements gave â€‰meV, â€‰meV, and â€‰meV [31]; (iii) the compound SmFeAsOF with â€‰K where, according to point-contact spectroscopy measurements, â€‰meV and â€‰meV [32, 33].

Inelastic neutron-scattering experiments suggest that the typical boson energy possibly responsible for superconductivity ranges roughly between 10 and 30â€‰meV [34, 35]. In the numerical simulations I used spectral functions with Lorentzian shape, that is, , where , are the normalization constants necessary to obtain the proper values of while and are the peak energies and half-widths, respectively. In all the calculations I always set , with ranging between 5 and 35 meV and â€‰meV. The cut-off energy is and the maximum quasiparticle energy is .

In the â€‰K case I know that and [36] while in the â€‰K case and [9] and in the â€‰K case I have and [37]. Once the energy of the boson peak is set, only two free parameters are left in the model: and .

By properly selecting the values of these parameters it is relatively easy to obtain the experimental values of the critical temperature and of the small gap, which is well known. It is more difficult to reproduce the values of the large gaps of bands 1 and 3 since, due to the high ratio (of the order of 8-9), high values of the coupling constants and small boson energies are required. Figures 2, 3, and 4 show the values of the calculated gaps (full symbols, left axis) as a function of the boson peak energy, . The corresponding values of and , chosen in order to reproduce the values of and of the small gap, , are also shown in the figure (open symbols, right axis). In all materials examined, only when â€‰meV the values of the large gap correspond to the experimental data. Indeed, when increases, the values of and strongly decrease. As a consequence, a rather small energy of the boson peak together with a very strong coupling (particularly in the 3-1 channel) is needed in order to obtain the experimental and the correct gap values. In this regard, it is worth noticing that the absolute values of the large gaps *cannot* be reproduced in a interband-only, two-band Eliashberg model [38], as well as within a three-band BCS model. In the latter case it is only possible to obtain a ratio of the gaps close to the experimental one [10, 11].

I also tested the effect into the model of a small intraband coupling (possibly of phonon origin). In the case of BaKFeAs (â€‰K) I fixed â€‰meV and since I know indeed that this coupling cannot be very high [5, 6]. Then I determined the free parameters and in order to obtain â€‰K. It might be thought that this term can sensibly contribute to increase the gap values but, as can be seen in Table 1, this is not the case as the gap values only show a slight increase.

The effect of Coulomb interaction was also investigated for the case shown in Table 1 where a weak intraband coupling is included. I chose and, as expected, I found that the intraband Coulomb pseudopotential has a negligible effect while the interband one [19] strongly contributes to raise and reduces in a considerable way [24] the value of . In this case, as shown in Table 1, it is only possible to obtain the correct value of the small gap because the electron-boson coupling is now too small and it is impossible to reproduce the value of the big gap. As a consequence, this result seems to exclude a strong interband Coulomb interaction in these compounds.

I also calculated the superconductive density of states in all three cases. The parameters used for the K case are â€‰meV, , and , for the â€‰K case â€‰mev, , and and for â€‰K case â€‰mev, , and .

The value of coupling constant is in the range 1â€“6 and this fact, at a first glance, may seem very unusual but these systems have some peculiarities in common with the heavy fermions superconductors. For example, in the compound LaFeAsOF, the normal state at is asymmetric and pseudogapped, with two broad maxima that are progressively smoothed out on increasing the temperature [30]. This shape is very similar to that observed by point contact spectroscopy in materials with long-range spin-density-wave order, like URuSi [39, 40]. The calculated superconductive normalized conductances are shown in Figure 5; the presence of a hump at is a typical strong coupling effect [41]. This feature, of course, is more evident when is bigger. By cause of thermal broadening it is impossible to separate the peaks of the gaps and .

The penetration depth as a function of temperature has been calculated in the three cases and is reported in Figure 6. It is in qualitative agree with the experimental data [42]. The inset shows the behaviour of at low temperature. Although at sufficiently low temperature an exponential fit may be certainly possible the inset shows that, on a larger range (up to ) these curves can be best fitted by a third-order polynomial as experimentally observed [42].

In conclusion, I have shown that the newly discovered iron pnictides very likely represent a case of dominant negative interband-channel pairing superconductivity where an electron-boson coupling, such as the electron-spin fluctuactions one, can become a fundamental ingredient to increase in a multiband strong-coupling picture. In particular, the present results prove that a simple three-band model in strong-coupling regime can reproduce in a quantitative way the experimental and the energy gaps of the pnictide superconductors with only two free parameters, and , provided that the typical energies of the spectral functions are of the order of 10â€‰meV and the coupling constants are very high ().

#### Acknowledgments

The author thanks I. I. Mazin for useful discussions, Mauro Tortello and Dario Daghero for manuscript revision.

#### References

- Y. Kamihara, T. Watanabe, M. Hirano, and H. Hosono, â€śIron-based layered superconductor $\text{La}[{\text{O}}_{1-x}{\text{F}}_{x}]\text{FeAs}(x=0.05-0.12)$ with ${T}_{c}=26\text{K}$,â€ť
*Journal of the American Chemical Society*, vol. 130, no. 11, pp. 3296â€“3297, 2008. View at Publisher Â· View at Google Scholar Â· View at PubMed Â· View at Scopus - Z.-A. Ren, W. Lu, J. Yang, et al., â€śSuperconductivity at 55 K in iron-based F-doped layered quaternary compound $\text{Sm}[{\text{O}}_{1-x}{\text{F}}_{x}]\text{FeAs}$,â€ť
*Chinese Physics Letters*, vol. 25, no. 6, pp. 2215â€“2216, 2008. View at Publisher Â· View at Google Scholar Â· View at Scopus - M. Rotter, M. Tegel, and D. Johrendt, â€śSuperconductivity at 38 K in the iron arsenide $({\text{Ba}}_{1-x}{\text{K}}_{x}){\text{Fe}}_{2}{\text{As}}_{2}$,â€ť
*Physical Review Letters*, vol. 101, no. 10, Article ID 107006, 2008. View at Publisher Â· View at Google Scholar Â· View at Scopus - C. de La Cruz, Q. Huang, J. W. Lynn, et al., â€śMagnetic order close to superconductivity in the iron-based layered ${\text{LaO}}_{1-x}{\text{F}}_{x}\text{FeAs}$ systems,â€ť
*Nature*, vol. 453, no. 7197, pp. 899â€“902, 2008. View at Publisher Â· View at Google Scholar Â· View at PubMed Â· View at Scopus - L. Boeri, O. V. Dolgov, and A. A. Golubov, â€śIs ${\text{LaFeAsO}}_{1-x}{\text{F}}_{x}$ an electron-phonon superconductor?â€ť
*Physical Review Letters*, vol. 101, no. 2, Article ID 026403, 4 pages, 2008. View at Publisher Â· View at Google Scholar Â· View at Scopus - L. Boeri, O. V. Dolgov, and A. A. Golubov, â€śElectron-phonon properties of pnictide superconductors,â€ť
*Physica C*, vol. 469, no. 9–12, pp. 628â€“634, 2009. View at Publisher Â· View at Google Scholar Â· View at Scopus - I. I. Mazin, D. J. Singh, M. D. Johannes, and M. H. Du, â€śUnconventional superconductivity with a sign reversal in the order parameter of ${\text{LaFeAsO}}_{1-x}{\text{F}}_{x}$,â€ť
*Physical Review Letters*, vol. 101, no. 5, Article ID 057003, 2008. View at Publisher Â· View at Google Scholar Â· View at Scopus - Physica C 469, 2009, Special Issue on Pnictides.
- I. I. Mazin and J. Schmalian, â€śPairing symmetry and pairing state in ferropnictides: theoretical overview,â€ť
*Physica C*, vol. 469, no. 9–12, pp. 614â€“627, 2009. View at Publisher Â· View at Google Scholar Â· View at Scopus - L. Benfatto, M. Capone, S. Caprara, C. Castellani, and C. di Castro, â€śMultiple gaps and superfluid density from interband pairing in a four-band model of the iron oxypnictides,â€ť
*Physical Review B*, vol. 78, no. 14, Article ID 140502, 4 pages, 2008. View at Publisher Â· View at Google Scholar Â· View at Scopus - E. Z. Kuchinskii and M. V. Sadovskii, â€śMultiple bands: a key to high-temperature superconductivity in iron arsenides?â€ť
*Journal of Experimental and Theoretical Physics Letters*, vol. 11, no. 3, pp. 156â€“160, 2009. View at Publisher Â· View at Google Scholar Â· View at Scopus - G. M. Eliashberg, â€śInteractions between electrons and lattice vibrations in a superconductor,â€ť
*Soviet Physycs. JETP Letters*, vol. 11, no. 3, pp. 696â€“702, 1960. - D. J. Scalapino, â€śThe Electron-phonon interaction and strong-coupling superconductors,â€ť in
*Superconductivity*, R. D. Parks, Ed., p. 449, Marcel Dekker, New York, NY, USA, 1969. - J. P. Carbotte, â€śProperties of boson-exchange superconductors,â€ť
*Reviews of Modern Physics*, vol. 62, no. 4, pp. 1027â€“1157, 1990. View at Publisher Â· View at Google Scholar Â· View at Scopus - P. B. Allen and B. Mitrovich, â€śTheory of superconducting ${T}_{c}$,â€ť in
*Solid State Physics*, H. Ehrenreich, F. Seitz, and D. Turnbull, Eds., vol. 37, Academic Press, New York, NY, USA, 1982. - F. Marsiglio and J. P. Carbotte, â€śElectron-phonon superconductivity,â€ť in
*The Physics of Conventional and Unconventional Superconductors*, K. H. Bennemann and J. B. Ketterson, Eds., p. 233, Springer, New York, NY, USA, 2003. - F. Marsiglio, â€śEliashberg theory of the critical temperature and isotope effect. Dependence on bandwidth, band-filling, and direct Coulomb repulsion,â€ť
*Journal of Low Temperature Physics*, vol. 87, no. 5-6, pp. 659â€“682, 1992. View at Publisher Â· View at Google Scholar Â· View at Scopus - C. R. Leavens and E. Talbot, â€śEffect of thermal phonons on the superconducting transition temperature,â€ť
*Physical Review B*, vol. 28, no. 3, pp. 1304â€“1313, 1983. View at Publisher Â· View at Google Scholar Â· View at Scopus - G. A. Ummarino, â€śEffects of magnetic impurities on two-band superconductor,â€ť
*Journal of Superconductivity and Novel Magnetism*, vol. 20, no. 7-8, pp. 639â€“642, 2007. View at Publisher Â· View at Google Scholar - S. V. Shulga, S.-L. Drechsler, G. Fuchs, et al., â€śUpper critical field peculiarities of superconducting ${\mathrm{YnI}}_{2}{B}_{2}\text{C}$ and ${\mathrm{LuNi}}_{2}{B}_{2}C$,â€ť
*Physical Review Letters*, vol. 80, no. 8, pp. 1730â€“1733, 1998. - S. D. Adrian, S. A. Wolf, O. V. Dolgov, S. Shulga, and V. Z. Kresin, â€śDensity of states and the energy gap in superconducting cuprates,â€ť
*Physical Review B*, vol. 56, no. 13, pp. 7878â€“7881, 1997. View at Publisher Â· View at Google Scholar - G. A. Ummarino, R. S. Gonnelli, S. Massidda, and A. Bianconi, â€śTwo-band Eliashberg equations and the experimental ${T}_{c}$ of the diboride ${\text{Mg}}_{1-x}{\text{AI}}_{x}{\text{B}}_{2}$,â€ť
*Physica C*, vol. 407, no. 3-4, pp. 121â€“127, 2004. View at Publisher Â· View at Google Scholar - E. J. Nicol and J. P. Carbotte, â€śProperties of the superconducting state in a two-band model,â€ť
*Physical Review B*, vol. 71, no. 5, Article ID 054501, 18 pages, 2005. View at Publisher Â· View at Google Scholar - G. A. Ummarino, â€śIron-based layered compounds: the effect of negative interband coupling,â€ť
*Journal of Superconductivity and Novel Magnetism*, vol. 22, no. 6, pp. 603â€“607, 2009. View at Publisher Â· View at Google Scholar - O. V. Dolgov, R. K. Kremer, J. Kortus, A. A. Golubov, and S. V. Shulga, â€śThermodynamics of two-band superconductors: the case of ${\text{MgB}}_{2}$,â€ť
*Physical Review B*, vol. 72, no. 2, Article ID 024504, 2005. View at Publisher Â· View at Google Scholar - D. Parker, O. V. Dolgov, M. M. Korshunov, A. A. Golubov, and I. I. Mazin, â€śExtended $s\pm $ scenario for the nuclear spin-lattice relaxation rate in superconducting pnictides,â€ť
*Physical Review B*, vol. 78, no. 13, Article ID 134524, 5 pages, 2008. View at Publisher Â· View at Google Scholar - H. J. Vidberg and J. W. Serene, â€śSolving the Eliashberg equations by means of N-point Padé approximants,â€ť
*Journal of Low Temperature Physics*, vol. 29, no. 3-4, pp. 179â€“192, 1977. View at Publisher Â· View at Google Scholar - C. R. Leavens and D. S. Ritchie, â€śExtension of the N-point Padé approximants solution of the Eliashberg equations to $\text{T}\sim {\text{T}}_{\text{C}}$,â€ť
*Solid State Communications*, vol. 53, no. 2, pp. 137â€“142, 1985. - G. A. Ummarino and R. S. Gonnelli, â€śReal-axis direct solution of the d-wave Eliashberg equations and the tunneling density of states in optimally doped ${\text{Bi}}_{2}{\text{Sr}}_{2}{\text{CaCu}}_{2}{\text{O}}_{8+x}$,â€ť
*Physica C*, vol. 328, no. 3, pp. 189â€“194, 1999. View at Publisher Â· View at Google Scholar - R. S. Gonnelli, D. Daghero, M. Tortello, et al., â€śCoexistence of two order parameters and a pseudogaplike feature in the iron-based superconductor ${\text{LaFeAsO}}_{1-x}{\text{F}}_{x}$,â€ť
*Physical Review B*, vol. 79, no. 18, Article ID 184526, 11 pages, 2009. View at Publisher Â· View at Google Scholar - H. Ding, P. Richard, K. Nakayama, et al., â€śObservation of Fermi-surface-dependent nodeless superconducting gaps in ${\text{Ba}}_{0.6}{\text{K}}_{0.4}{\text{Fe}}_{2}{\text{As}}_{2}$,â€ť
*Europhysics Letters*, vol. 83, no. 4, Article ID 47001, 2008. View at Publisher Â· View at Google Scholar - D. Daghero, M. Tortello, R. S. Gonnelli, V. A. Stepanov, N. D. Zhigadlo, and J. Karpinski, â€śEvidence for two-gap nodeless superconductivity in ${\text{SmFeAsO}}_{1-x}{\text{F}}_{x}$ from point-contact Andreev-reflection spectroscopy,â€ť
*Physical Review B*, vol. 80, no. 6, 2009. View at Publisher Â· View at Google Scholar - D. Daghero, M. Tortello, R. S. Gonnelli, et al., â€śPoint-contact Andreev-reflection spectroscopy in ${\text{ReFeAsO}}_{1-x}{\text{F}}_{x}(\text{Re}=\text{La,Sm})$: possible evidence for two nodeless gaps,â€ť
*Physica C*, vol. 469, no. 9–12, pp. 512â€“520, 2009. View at Publisher Â· View at Google Scholar - A. D. Christianson, E. A. Goremychkin, R. Osborn, et al., â€śUnconventional superconductivity in ${\text{Ba}}_{0.6}{\text{K}}_{0.4}{\text{Fe}}_{2}{\text{As}}_{2}$ from inelastic neutron scattering,â€ť
*Nature*, vol. 456, no. 7224, pp. 930â€“932, 2008. View at Publisher Â· View at Google Scholar Â· View at PubMed Â· View at Scopus - R. Osborn, S. Rosenkranz, E. A. Goremychkin, and A. D. Christianson, â€śInelastic neutron scattering studies of the spin and lattice dynamics in iron arsenide compounds,â€ť
*Physica C*, vol. 469, no. 9–12, pp. 498â€“506, 2009. View at Publisher Â· View at Google Scholar Â· View at Scopus - M. V. Sadovskii, â€śHigh-temperature superconductivity in iron-based layered iron compounds,â€ť
*Physics-Uspekhi*, vol. 51, no. 12, pp. 1201â€“1227, 2008. View at Publisher Â· View at Google Scholar Â· View at Scopus - I. I. Mazin, private communication.
- O. V. Dolgov, I. I. Mazin, D. Parker, and A. A. Golubov, â€śInterband superconductivity: contrasts between Bardeen-Cooper-Schrieffer and Eliashberg theories,â€ť
*Physical Review B*, vol. 79, no. 6, Article ID 060502, 2009. View at Publisher Â· View at Google Scholar Â· View at Scopus - K. Hasselbach, J. R. Kirtley, and P. Lejay, â€śPoint-contact spectroscopy of superconducting ${\text{URu}}_{2}{\text{Si}}_{2}$,â€ť
*Physical Review B*, vol. 46, no. 9, pp. 5826â€“5829, 1992. View at Publisher Â· View at Google Scholar Â· View at Scopus - R. Escudero, F. Morales, and P. Lejay, â€śTemperature dependence of the antiferromagnetic state in ${\text{URu}}_{2}{\text{Si}}_{2}$ by point-contact spectroscopy,â€ť
*Physical Review B*, vol. 49, no. 21, pp. 15271â€“15275, 1994. View at Publisher Â· View at Google Scholar Â· View at Scopus - G. A. Ummarino, R. S. Gonnelli, and D. Daghero, â€śTunneling conductance of SIN junctions with different gap symmetries and non-magnetic impurities by direct solution of real-axis Eliashberg equations,â€ť
*Physica C*, vol. 377, no. 3, pp. 292â€“303, 2002. View at Publisher Â· View at Google Scholar - R. Prozorov, M. A. Tanatar, R. T. Gordon, et al., â€śAnisotropic London penetration depth and superfluid density in single crystals of iron-based pnictide superconductors,â€ť
*Physica C*, vol. 469, no. 9–12, pp. 582â€“589, 2009. View at Publisher Â· View at Google Scholar